Published online September 30, 2014 (http://www.sciencepublishinggroup.com/j/ijmsa) doi: 10.11648/j.ijmsa.20140305.30

ISSN: 2327-2635 (Print); ISSN: 2327-2643 (Online)

**A theoretical study of the heavy and light hole properties **

**of Cd**

**1-x**

**Zn**

**x**

**S quantum dot superlattices **

**Saber Marzougui, Nabil Safta**

*****

Unité de Physique Quantique, Faculté des Sciences, Université de Monastir, Monastir, Tunisia

**Email address: **

[email protected] (N. Safta)

**To cite this article: **

Saber Marzougui, Nabil Safta. A Theoretical Study of the Heavy and Light Hole Properties of Cd1-xZnxS Quantum Dot Superlattices.

*International Journal of Materials Science and Applications. *Vol. 3, No. 5, 2014, pp. 274-278. doi: 10.11648/j.ijmsa.20140305.30

**Abstract:**

This work reports on a theoretical investigation of superlattices based on Cd1-xZnxS quantum dots embedded in
an insulating material. This system, considered as a series of flattened cylindrical quantum dots with a finite barrier at the boundary, is studied using the tight binding approximation. The ground miniband width and the longitudinal effective mass, in the case of the heavy and light holes, have been computed as a function of zinc composition for different inter-quantum dot separations. An analysis of the results shows that the Zn composition x = 0.8 are appropriate to give rise a superlattice behavior for the light holes. As for the heavy holes, it has been showed the strong localization character of theses carriers in the Cd1-xZnxS nanostructures.

**Keywords:**

Quantum Dots, Superlattices, Cd1-xZnxS, Heavy and Light Holes, Tight Binding Approximation,
Specific Devices

**1. Introduction **

In the last decades, films of Cd1−xZn*x*S have found wide

applications in electrical, optical and electro – optical devices [1-3].The high potentialities of these films is mainly due to their utility as window materials in heterojunction solar cells with a p-type absorber like CuInSe2,CuInxGa1-xSe2 or CuSnSz Se1-z [4-6]. On the other

hand, Cd1−xZn*x*S thin films have led to a decrease in

window absorption and to an increase in the short circuit current as well [7-9].

To the subject of Cd1−xZn*x*S quantum dots (QDs), their

considerable interest has been proved in both fundamental and applied research [4, 10-20]. For our part, we have adopted, in a first time, the spherical geometry with a finite potential barrier at the boundary to describe the Cd1-xZnxS

QDs [21, 22]. Thus, by restricting the study to the ground state for both electrons and holes, we have calculated, in a first step, the shape of the confinement potentials, the quantized energies, their related envelope wave – functions and the QDs sizes [21]. We have calculated, in a second step, for electrons and holes, the excited bound states [22]. All these calculations have been made versus the zinc composition.

We have suggested, in a second time, the flattened

cylindrical geometry with a finite potential barrier at the boundary [23-29]. Using this model, we have investigated, in a first step, the electronic properties of Cd1-xZnxS

quantum dots [23]. More precisely, we have calculated the shape of the confining potential, the subband energies and their eigen envelope wave functions. We have studied, in a second step, the coupling in the case of superlattices based on Cd1-xZnxS quantum dots embedded in an insulating

material with use of several potential models and different methods (Kronig – Penney method, sinusoidal and triangular potentials, Tight Binding approximation…) [24-29]. In this context, our interest has been focused, in a recent study, on the computation of the ground miniband width and the longitudinal effective mass for the electrons. Calculations have been made versus the ZnS molar fraction for different superlattice periods with use of the Tight Binding approximation (TBA) [28]. From this study, we have deduced that the Zn compositions x = 0.4 and x = 0.6 are appropriate to give rise a superlattice behavior for conduction electrons. As for the longitudinal electron effective mass, it is found to be the lower for x = 0.4 and x = 0.6 [28].

presented in the last part.

**2. Theoretical Details **

Fig. 1- a depicts the geometry used to describe a chain of Cd1-xZnxS QDs. The common confined direction is denoted

by z. The inter-quantum dot separation is labelled d which corresponds to the period of the structure. Along a common direction of spherical Cd1-xZnxS QDs, electrons and holes

see a succession of flattened cylinders of radius R and effective height L. If we consider L = 1 nm [23] and the fact that the diameter D = 2R varies from 9 nm to 4 nm going from CdS to ZnS [4] it clearly appears that L is lower than D. Consequently the quantum confinement along transversal direction can be disregarded and the Cd1-xZnxS

multi – quantum dot system being studied can be considered as a QDs superlattice along the longitudinal confined direction. Thus,the system toinvestigate is a Cd 1-xZnxS QD superlattice where the Cd1-xZnxS flattened

cylinders QDs correspond to wells while the host dielectric
lattice behaves as a barrier of height *U0*. For the sake of

simplicity, the electron and hole states are assumed to be uncorrelated. The problem to solve is, then, reduced to those of one particle in a one dimensional potential. In this work, we consider the potential depicted in Fig. 1- b. Such a potential can be expressed as:

### ( )

=### ∑

### (

### )

*n*
*e,h*

*e,h* *z* *U* *z - nd*

*V* (1)

with

### ( )

- 2 22 2 ; 0

0 *; - L/* *z* *L/*

*U*

*d-L/*
*z*
*L/*
*z*

*U _{e,h}* =

*e,h*<

_{<}<

_{<}

The subscripts *e* and *h* refer to electrons and holes
respectively and n is the nth period. For this potential, the
electron and hole states can be calculated using the
effective Hamiltonian:

## ( )

*e,h*

*e,h*

*e,h*

***

*e,h*

*e,h* * V* *z*

*dz*
*d*

*m*

*H* = − +

2 2 2 2 ℏ (2)

where ℏ is the Plank’s constant and *m** is the effective

mass of carriers. In deriving the Hamiltonian *He,h*, we have

adopted the effective mass theory (EMT) and the band parabolicity approximation (BPA). The difference of the effective mass between the well and the barrier has been neglected.

We have resolved the Schrodinger equation using the
Tight Binding Approximation. A peculiar attention is paid
to the longitudinal dispersion relation which shows the
k-dependence of minibands along the [001] direction. If we
neglect the wave function overlap, this relation is given, in
the case of the ground miniband (*Γ*_{1} −miniband), by [28]:

### ( )

*k*

### (

*E*

*U*

### )

### ( )

*k*

*d*

*E _{e}*

_{,}

_{h}*=*

_{z}_{1}

_{e}_{,}

*−*

_{h}_{0}

_{e}_{,}

*+2γ*

_{h}

_{e}_{,}

*+2β*

_{h}

_{e}_{,}

*cos*

_{h}*(3)*

_{z}Here, *E1e* corresponds to the lowest energy of electrons and

*E1h* is the lowest energy of holes (*E1h*≡*E1hh* for heavy holes

and *E1h* ≡ *E1lh *for light holes). All these energies are

associated with an isolated flattened cylindrical quantum dot of Cd1-xZnxS and calculated in such a way that the zero

energy is taken at the bottom of the QD well [23, 29].

**Figure 1. ***(a) A schematic diagram of Cd1-xZnxS QD superlattices *

*according to the flattened cylindrical geometry – (b) The barrier potential *
*in the framework of the Tight Binding Approximation . *

*βe* and γ*e* are respectively, the exchange and the

correlation integrals. These parameters are, respectively,
given by:
+
+
−
−
−
=
2
,
2
,
sin
,
2
,
2
,
cos
,
2
,
2
,
2
,
,
,
,
0
2
,
*L*
*h*
*e*
*ch*
*L*
*h*
*e*
*k*
*h*
*e*
*k*
*L*
*h*
*e*
*sh*
*L*
*h*
*e*
*k*
*h*
*e*
*h*
*e*
*k*
*h*
*e*
*L*
*d*
*h*
*e*
*e*
*h*
*e*
*B*
*h*
*e*
*A*
*h*
*e*
*U*
*h*
*e*
ρ
ρ
ρ
ρ
ρ
β
_{−}
−

= _{2},

,
2
,
,
,
0
,
2 _{L}*h*
*e*
*sh*
*h*
*e*
*d*
*L*
*h*
*e*
*e*
*h*
*e*
*B*
*h*
*e*
*U*
*h*
*e*
ρ
ρ
ρ
γ
with

### ( )

21
,
,
,
,
2
,
2
sin
2
cos
2
−
+
+
=
*h*
*e*
*h*
*e*
*h*
*e*
*h*
*e*
*h*
*e*
*k*
*L*
*k*
*L*
*k*
*L*
*A*
ρ
=
2
cos ,
,
,
*L*
*k*
*A*

*B _{e}_{h}*

_{e}_{h}*eh*

### (

### )

2 1 0 2 1 2 ; 2 ℏ ℏ*e,h*

*e,h*

***

*e,h*

*e,h*

*e,h*

***

*e,h*

*e,h*

*E*

*U*

*m*

*ρ*

*E*

*m*

*k* = = −

**3. Results and Discussion **

summarized in Table 1. All these parameters are taken from Refs [23, 29]. Values of the effective masses of the heavy and light holes for Cd1-xZnxS with different Zn

compositions have been deduced using the Vegard’s law.

**Table 1.** Parametersused to calculate the Γ_{1}*- miniband in the case of the *
*heavy and light holes for Cd1-xZnxS QD superlattices.*

**x **

0

*m*
*m*hh*

0
*m*
*m* _{lh}*

**U****0h****(eV) ** **L****(nm) ** *E*1*hh*( )eV *E*1*lh*( )eV

0.0 5.00 0.70 0.25 1.00 0.040 0.129 0.2 0.25 1.00 0.049 0.136 0.4 0.50 1.00 0.060 0.216 0.6 0.50 1.00 0.070 0.238 0.8 0.50 1.00 0.083 0.266 1.0 1.76 0.23 2.00 1.00 0.145 0.538

One can easily deduce, from (3), that the *Γ*1*h*- miniband
width is given by:

*h*

*E*_{1}

∆ =4

### β

*h*(4)

Thus, we have carried out this parameter for all the compositions and superlattice periods studied. Typical results are reported in Table 2 and Table 3.

**Table 2.***The Γ*_{1} *- miniband width ( 10-3 _{ eV), as calculated for the heavy }*

*holes versus the ZnS molar fraction for different inter-QD separations. *

**d (nm)** **1.5** **1.7** **1.9** **2.1** **2.3** **2.5**

**x **

0.2 7.628 3.059 1.174 4.507 0. 173 0. 066 0.4 3.596 0.973 0.263 0.071 0. 193 0. 005 0.6 6.533 2.020 6.248 0. 193 0. 059 0. 018 0.8 16.31 4.312 1.546 0. 554 0. 198 0. 071 1.0 1.887 0.029 0. 046 0. 037 0. 001 0. 002

This study led, for the light holes, to several observations:

(i) ∆*E*_{1}* _{lh}*shows a decreasing tendency when d increases
independently of the Zn composition. As a consequence,
the coupling decreases as the inter – quantum dot
separation increases (ii) for Cd1-xZnxS QDs with x = 0; 0.2

and 0.4, ∆*E*_{1}* _{lh}*is globally low (iii) for ZnS QD superlattices,

*lh*

*E*_{1}

∆ shows a drastic drop as the inter – quantum dot separation increases. Thus, the coupling is very weak at high SL periods. In this case, Cd1-xZnxS nanocrystallites are

nearly isolated (iv) for x = 0.8, ∆*E*_{1}* _{lh}* is maximum
independently of the inter-quantum dot separation. This
reflects the strong degree of coupling between the QDs.
Since the well width L being the same for all Zn
compositions, these results are, most probably, related to

the barrier potential height*U*_{0}* _{h}*, the bulk effective mass

***
*lh*

*m* and the energy *E1lh *values (v) For Cd1-xZnxS QDs with

x = 0.6, the magnitude order of ∆*E*_{1}* _{lh}*is not far from the one
of x = 0.8.

The comparison with results obtained for electrons [28]

shows that ∆*E*_{1}* _{lh}*is, globally, slightly lower than the

*Γ*

_{1}- miniband width for electrons (Table 4). Therefore, the superlattice behavior affects not only the conduction electrons but also the light holes especially for short SL periods.

As for the heavy holes, ∆*E*_{1}* _{hh}*is insignificant in terms of
magnitude order which means that the strong localization
character of heavy holes in the SL systems is totally
preserved going from CdS to ZnS independently to the SL
periods. As a consequence, we can consider that there is no
formation of minibands.

**Table 3.***The Γ*_{1} *- miniband width (eV), as calculated for the light holes *
*versus the ZnS molar fraction for different inter-QD separations. *

**d (nm)** **1.5** **1.7** **1.9** **2.1** **2.3** **2.5**

**x **

0.2 0.190 0.115 0.088 0.067 0.053 0. 039 0.4 0.187 0.126 0.085 0.058 0. 039 0. 026 0.6 0.236 0.174 0.117 0. 083 0. 059 0. 042 0.8 0.313 0.217 0.164 0. 123 0. 091 0. 070 1.0 0.301 0.173 0.095 0. 052 0. 029 0. 016

**Table 4.** The Γ_{1} *- miniband width, as calculated for electrons versus the *
*ZnS molar fraction for different inter-QD separations[28]. *

**d (nm)** **1.5** **1.7** **1.9** **2.1** **2.3** **2.5**

**x **

0.0 0.056 0.054 0.052 0.050 0.048 0.046 0.2 0.211 0.189 0.169 0.151 0.135 0.121 0.4 0.352 0.294 0.242 0.201 0.167 0.139 0.6 0.406 0.302 0.224 0.166 0.123 0.091 0.8 0.344 0.208 0.125 0.076 0.045 0.027 1.0 0.241 0.126 0.065 0.034 0.017 0.009

Concerning the longitudinal effective mass of light holes
***

*lh,Γ*

*m*

1

, we can write [28]:

***
*lh,Γ*

*m*

1 2

2

2β* _{lh}d*
ℏ

= _{ (5) }

We have calculated this parameter, in the case of the light holes, versus composition x for the different inter – QD separations studied. All these effective masses are expressed in units of the free electron mass m0. Results are

reported in Table 5.

**Table 5. **The longitudinal effective mass calculated, for the light holes, as *a function of the inter-sheet separation for Cd1-xZnxS QD superlattices *

**d(nm)** **1.5** **1.7** **1.9** **2.1** **2.3** **2.5**

**x **

An analysis of the obtained results revealed: (i) *m* _{lh,Γ}*

1

shows an increasing tendency when d increases independently of the Zn composition. Therefore, the light hole mobility is expected to be decreasing with increased d (ii) for Cd1-xZnxS QDs with x = 0; 0.2 and 0.4,

***
*lh,Γ*

*m*

1

values are globally high (iii) for ZnS QD superlattices,
***

*lh,Γ*

*m*

1

values are rather high for large SL periods. In this

case, the transport of light holes is significantly reduced (iv)
for x = 0.8, the order of magnitude of *m* _{lh,Γ}*

1 is low

independently of the inter-quantum dot separation. It is of particular interest that, for this composition, the SL period does not significantly affect the transport properties (v) For Cd1-xZnxS QDs with x = 0.6,

***
*lh,Γ*

*m*

1 is slightly higher than

the one of x = 0.8.

It should be noted that, for the heavy holes, the Cd

1-xZnxS nanoparticles behave as isolated QDs. The effective

mass being related to the miniband dispersion can not be defined in such a case.

**4. Conclusion **

We investigated the coupling in superlattices made by Cd1-xZnxS QDs for compositions ranging from CdS to ZnS.

To describe the QDs, we have proposed the flattened
cylindrical geometry with a finite potential barrier at the
boundary. Using the Tight Binding Approximation, we
have calculated, in a first step, for the heavy and light holes
the *Γ*_{1} - miniband. Calculations have been made as a
function of Zn composition for different inter – quantum
dot separations.

An analysis of the obtained results has evidenced that the Zn composition x = 0.8 are appropriate to give rise a superlattice behavior for the light holes. As for the heavy holes, the results showed the strong localization character of theses carriers in the Cd1-xZnxS nanostructures.

Concerning the longitudinal effective mass of the light holes, it is found to be the lower for x = 0.8.

In the applied physics, this study open a new way for designing specific devices based on well controlled Cd

1-xZnxS QDs especially the non – volatile memories.

**References **

[1] A. Sakly, N. Safta and A. Ben Lamine. (2004), Interpretation of the bowing phenomenon in Cd1-xZnxS alloy, J. Mater.

Sci.-Mater. Electron. 15 : 351.

[2] N. A. Shah, A. Nazir, W. Mahmood, W. A. Syed, S. Butt, Z. Ali and A. Maqsood. (2012), Physical properties and characterization of Ag doped CdS thin films, J. Alloys Compd. 512: 27.

[3] T. P. Kumar, S. Saravanakumar and K. Sankaranayanan. (2011), Effect of annealing on the surface and band gap alignment of CdZnS thin films, Appl. Surf. Sci. 257 (6) :

1923.

[4] B. Bhattacharjee, S. K. Mandal, K. Chakrabarti, D. Ganguli and S. Chaudhui. (2002), Optical properties of Cd1−xZnxS nanocrystallites in sol–gel silica matrix, J. Phys. D: Appl. Phys. 35: 2636-2642.

[5] H. H. Gürel, Ö. Akinci and H. Ünlü. (2008), Tight binding modeling of CdSe/ZnS and CdZnS/CdS II–VI heterostructures for solar cells: Role of d-orbitals, Thin Solid Films 516 : 7098.

[6] M. Gunasekaram, M. Ichimura. (2007), Photovoltaic cells based on pulsed electrochemically deposited SnS and photochemically deposited CdS and Cd1−xZnxS, Sol. Energy Mater. Sol. Cells. 91 : 774.

[7] N. Kohara, T. Negami, M. Nishitani and T. Wada. (1995), Preparation of Device – Quality Cu (In, Ga)Se2 Thin films

deposited by Coevaporation with composition Monitor, Japan. J. appl. Phys. 34 : L 1141

[8] V. Alberts, R. herberhonz, T. Walter and H. W. Schock. (1997), Device characteristics of In-rich CuInSe2 based solar

cells, J. Phys. D: Appl. Phys. 30 : 2156.

[9] J. Lee, W. Song and J. Yi. (2003), Growth and properties of the Cd1-xZnxS films for solar cell applications, Thin Solid

Films 431-432 : 349.

[10] A. J. Peter and C. W. Lee.(2012), Electronic and optical properties of CdS/CdZnS nanocrystals, Chinese Phys. B 21: 087302.

[11] F. Scotognella, G. Lanzani, L. Manna, F. Tassone and M. Zavelani-Rossi. (2012), Study of higher-energy core states in CdSe/CdS octapod nanocrystals by ultrafast spectroscopy, Eur. Phys. J. B. 85: 128.

[12] L. Cao, S. Huang and S. E. (2004), ZnS/CdS/ZnS quantum dot quantum well produced in inverted micelles, J. colloid Interface Sci. 273: 478-482.

[13] H. Kumano, A. Ueta and I. Suemune. (2002), Modified spontaneous emission properties of CdS quantum dots embedded in novel three-dimensional microcavities, Physica E 13: 441-445

[14] Y. C. Zhang, W. W. Chen and X. Y. Hu. (2007), In air synthesis of hexagonal Cd1 − xZnxS nanoparticles from

single-source molecular precursors, Mater. Lett. 61: 4847-4850

[15] C. S. Pathak, D. D. Mishra, V. Agarawala, M. K. Mandal. (2012), Mechanochemical synthesis, characterization and optical properties of zinc sulphide nanoparticles, Indian J. Phys 86: 777-781.

[16] S. Roy, A. Gogoi and G. A. Ahmed. (2010), Size dependent optical characterization of semiconductor particle: CdS embedded in polymer matrix, Indian J. Phys. 84: 1405-1411

[17] A. U. Ubale and A. N. Bargal. (2010), Characterization of nanostructured photosensitive cadmium sulphide thin films grown by SILAR deposition technique, Indian J. Phys. 84: 1497-1507

[19] N. Safta. (2004), Fluctuations mode of the gap as a function of composition of Cd1-xZnxS ternaries, Ann. Chim. Sci. Mat. 29 (5) 105-112

[20] H. Yükselici, P. D. Persans and T. M. Hayes.(1995), Optical
studies of the growth of Cd1-*x*Zn*x*S nanocrystals in
borosilicate glass, Phys. Rev. B. 52: 11763.

[21] N. Safta, A. Sakly, H. Mejri and Y. Bouazra. (2006), Electronic and optical properties of Cd1-xZnxS nanocrystals,

Eur. Phys. J. B 51: 75-78

[22] A. Sakly, N. Safta, A. Mejri, H. Mejri, A. Ben Lamine. (2010), The Excited Electronic States Calculated for

*Cd1-x*Zn*x*S Quantum Dots Grown by the Sol-Gel Technique,
J. Nanomater, ID746520.

[23] N. Safta, A. Sakly, H. Mejri and M. A. Zaïdi. (2006), Electronic properties of multi-quantum dot structures in Cd 1-xZnxS alloy semiconductors, Eur. Phys. J. B 53: 35 – 38

[24] A. Sakly, N. Safta, H. Mejri, A. Ben Lamine. (2009), The electronic band parameters calculated by the Kronig–Penney method for Cd1−xZnxS quantum dot superlattices, J. Alloys

Compd. 476: 648–652.

[25] A. Sakly, N. Safta, H. Mejri, A. Ben Lamine. (2011), The electronic states calculated using the sinusoidal potential for Cd1−xZnxS quantum dot superlattices, J. Alloys Compd.509:

2493–2495

[26] S. Marzougui, N. Safta. (2014), The electronic band parameters calculated by the Triangular potential model for Cd1-xZnxS quantum dot superlattices, IOSR-JAP 5 (5) :

36-42

[27] S. Marzougui, N. Safta. (2014), The electronic band parameters calculated by the Tight Binding Approximation for Cd1-xZnxS quantum dot superlattices, IOSR-JAP 6 (2) :

15-21

[28] S. Marzougui,N. Safta. (2014), A theoretical study of the electronic properties of Cd1-xZnxS quantum dot superlattices,

*American Journal of Nanoscience and Nanotechnology* 2
(3) : 45-49.

[29] S. Marzougui. (2011), *A study of the excited states in the *
*flattened cylindrical quantum dots of Cd1-xZnxS*, Master,